1 26 Rev.Adv.Mater.Sci. 24(2010) O. Maksimov RECENT ADVANCES AND NOVEL APPROACHES OF P-TYPE DOPING OF ZINC OXIDE Oleg Maksimov Materials Research Institute, Pennsylvania State University, University Park, PA Received: January 02, 2010 Abstract. Due to its high radiative stability and superior optoelectronic properties, such as wide direct band gap of ~3.4 ev and high exciton binding energy of ~60 mev, ZnO is considered for the fabrication of ultraviolet and visible light emitting and laser diodes, solar-blind photodetectors. Although proof-of-concept devices were already demonstrated, further progress in this area is slowed down by the difficulties of doping ZnO p-type. Here, we discuss problems associated with doping of ZnO, cover recent progress in this area, and discuss an alternative approach to increase p-type dopability via anion substitution, replacing oxygen with other group VI elements (S, Se, Te). We also propose that these anion-substituted alloys will be extremely promising for fabrication of photovoltaic devices, such as highly efficient thin film solar cells. 1. PROPERTIES AND GROWTH OF ZnO There is significant technological and scientific interest in zinc oxide (ZnO) due to its unique physical and chemical properties . It is radiatively hard wide band gap semiconductor (E G ~3.37 ev) that can be easily doped n-type. Its band gap energy can be tuned by alloying with MgO and CdO from 7.9 ev to 2.3 ev , spanning from deep ultraviolet (UV) to visible regions of the spectrum. It has a higher exciton binding energy (E b of ~60 mev) than other wide band gap semiconductors like GaN and SiC, leading to the efficient excitonic transitions at room temperature. In addition, owing to the availability of native substrates 1 and amenability to wet chemical etching, ZnO is an extremely promising material for the development of optoelectronic devices, such as Corresponding author: Oleg Maksimov, light emitting and laser diodes (LEDs and LDs) and solar-blind photo detectors, and transparent thin film transistors. ZnO nanostructures (nanoparticles, nanorods, nanobelts, etc.), which can be synthesized using inexpensive physical vapor transport techniques, were shown to be extremely promising for the application as gas sensors, due to the large surface to volume ratio , and microlasers due to the superior optical properties . Furthermore, reports of high-temperature ferromagnetism in ZnO doped with transition metals (known as dilute magnetic oxide semiconductor)  coupled with nanosecond-long spin coherence time measured at low temperatures  makes this material extremely promising for future application in spin electronics (spintronics). 2 For comparison of ZnO with other wide band gap semiconductors see Table 1. 1 Wafers with the diameter up to 4 inches are available from a number of companies including Cermet Inc., MTI Corporation, and Zn Technology Inc. 2 Use of quantum mechanical spin states associated with the charged particles to propagate information offers potential advantages over the use of charge alone, as in present-day technology. Spintronic devices, combining the advantages of magnetic metals and semiconductors, are expected to be non-volatile, versatile, fast, capable of simultaneous data storage and processing, and power efficient. They can be used in high-density data recording and storage, quantum computation, cryptography, and microelectronic.
2 Recent advances and novel approaches of p-type doping of zinc oxide 27 Table 1. Physical properties of wide band gap semiconductors. Semiconductor Crystal Structure Band gap E G (ev) at ~ 6K E b (mev) ZnO Wurzrite Direct ZnS Zincblende Direct ZnSe Zincblende Direct ZnTe Zincblende Direct GaN Wurzrite Direct H-SiC Wurzrite Indirect Table 2. Best parameters reported for ZnO films. <0002> <10-11> FWHM of band electron density electron mobility peak peak edge emission at room at room at 10K temperature temperature Units degree degree mev cm -3 cm 2 V -1 s -1 Parameter >0.01 > mev 5 x Growth PLD PLD MBE PLD PLD Technique Substrate ScAlMgO 4 ScAlMgO 4 GaN ScAlMgO 4 ScAlMgO 4 Reference [27,81] [27,81]    High crystalline quality ZnO films are successfully deposited using a number of growth platforms, including molecular beam epitaxy (MBE), chemical vapor deposition (CVD), pulsed laser deposition (PLD), and reactive sputtering. Elemental sources (Zn and ozone or oxygen plasma), ceramic targets (ZnO), and metalorganic precursors (dimethylzinc and diethylzinc) are used with equal success. The best parameters reported for the ZnO films are shown in Table 2. Some of these growth techniques, such as PLD, can be used to deposit films and device structures only on the small wafers, up to 1 inch in diameter, and are more applicable for academic research. Others, such as sputtering, are easily scalable and allow straightforward integration with modern microelectronic industry. 2. P-TYPE DOPING OF ZnO However, further progress in this area is stalled by the difficulties of doping ZnO p-type. It is generally acknowledged that high enough doping levels are difficult to achieve both due to the background n- type doping originating from the presence of H impurities , O vacancies (V O ) , and Zn interstitials (Zn i ) , and due to the large acceptor activation energies and / or low solubility of commonly used group-v (N, P, As, Sb) and group I (Li) dopants. In addition, a slow transition from p-type to n-type conductivity was observed by a number of groups. It was tentatively assigned either to the acceptor migration from the substitutional to the interstitial position and / or to the hydrogen diffusion [10,11]. In spite of these difficulties, there are reports of ZnO doped p-type with group V (N [12,13] P [14,15], As [16-20], and Sb [21,22]), and group I (Li ) elements. Co-doping with two potential acceptors (N and As)  or acceptor and donor (N and Al) [25,26] was also studied. In the case of the acceptor-donor co-doping, the improvement is believed to be primarily due to the higher solubility of the forming N-Al-N complex. A temperature modulation epitaxy technique was also applied to achieve N-doped p-type ZnO . Nitrogen-doped layers were grown followed by the deposition of thin undoped layers at quality. In addition, doping with other elements, such as Ag and Bi, was explored [28,29]. These results are summarized in Table 3. Unfortunately, most of these results were extremely challenging to reproduce and nontrivial to interpret. For example, ZnO films grown by PLD on GaAs substrates were reported to be p-type. This was explained by the As diffusion from the GaAs substrate into the ZnO layer . However, addi-
3 28 O. Maksimov Table 3. Summary of attempts to grow p-type doped ZnO films. Dopant Growth N A (cm -3 ) (cm 2 / V s) P (Ohm cm) Reference Technique N CVD 1.06x  N CVD ZnO:N remained n-type  P Diffusion ZnO:P layer was p-type  P Sputtering 1.9x x  As PLD  As Sputtering 9x  As PLD 2.4x x  As CVD 1.45x  As PLD 4x  Sb MBE 1x  Sb PLD 1.9x  Li PLD 6.04x  N + As CVD Mixed conductivity  N + Al Sputtering 2.52x  N + Al Sputtering 1.45x  N PLD 8  Ag PLD 4.9x x  Bi MBE ZnO:Bi remained n-type  tional effects, such as formation of an interfacial Zn 2 As 2 O 7 layer , Ga diffusion into the ZnO film [31,32], and Zn diffusion into the GaAs substrate  were reported by other groups. In addition, isolated As atoms should act either as deep acceptors (As is incorporated substitutionally at the O position - As O ) and donors (As is incorporated substitutionally at the Zn position - As Zn ) or remain amphoteric (As is incorporated interstitially - As i ). Thus, p-type conductivity was explained by the formation of a complex with two spontaneous Zn vacancies (As Zn -2V Zn ) . Clearly, data interpretation was not straightforward and the origin of the p-type response remained controversial. Due to the difficulties with achieving highly p-type doped ZnO, proof of concept devices that did not employ p-type ZnO layer, such as n-zno/p-srcu 2 O 2 , n-zno/p-sic , n-zno/p-si , ZnO-based metal-insulator-semiconductor , n-gan/zno nanowire/p-gan , and n-zno/p-gan were fabricated [40,41]. The last approach was widely explored due to the low lattice mismatch between ZnO and GaN and possibility of band gap engineering using Al x Ga 1-x N alloy. Thus, p-al x Ga 1-x N/ZnO/n- Mg x O LEDs operating at high temperatures, up to 650K, were demonstrated . In addition, there were a few recent reports on the fabrication of homojunction LEDs, indicating continuous progress in this area [43-47]. ZnO-based LEDs produced using spray pyrolysis were particularly promising . Possibility to use such a low-cost and easily scalable technique justifies further development of this material system. Results of these research efforts are summarized in Table 4. In addition, ZnO-based UV photo detectors - another important area of ZnO application - were demonstrated by a number of research groups [49-51]. These devices are promising for the fabrication of the early warning missile defense systems, can be used for high temperature flame detection, for the monitoring of ozone layer, and in solar astronomy. However, homojunction LEDs suffered from high turn-on-voltage, reaching 12 V in the case of Be x O-based LED, and strong deep level defect-related emission. While high turn-on-voltage can be explained by the significant resistivity of the p-type layer, deep level emission may arise due to the inferior crystalline quality of the p-type layer. Although there are reports that a large dopant concentration can be incorporated into ZnO without degradation of a crystalline quality [52,53], a poorer in-plane and out-of-plane aliment, larger tilt and twist, is often observed . This may be due both to the defects
4 Recent advances and novel approaches of p-type doping of zinc oxide 29 Table 4. Characteristics of ZnO-based LEDs. n-layer p-layer (nm) Turn-on voltage (V) Reference ZnO SrCu 2 O  ZnO:Al 4H-SiC  ZnO Si 385 Under reverse bias  ZnO 380,  GaN:Si GaN:Mg 382,  ZnO:Ga GaN:Mg  ZnO:Ga GaN:Mg  Mg x O Al y Ga 1-y N  ZnO ZnO:N Operate only below 200K  Be x O:Ga Be x O:As 363, 388,  ZnO ZnO:N 423,  ZnO ZnO:As 388,  ZnO ZnO:N  Mg x O Mg x O:N+In 450,  introduced by the dopant, such as acceptor taking interstitial position (P i, As i, Sb i ) pared with the formation of oxygen vacancy (V O ), as well as to the lower growth temperatures used to increase solubility. Therefore, a novel approach is clearly needed to achieve high crystalline quality p-type ZnO layers necessary for the fabrication of low turn-on-voltage LEDs, LDs, and p-n junction photo detectors. 4. GROWTH AND DOPING OF ANION SUBSTITUTIED ZnO It was recently suggested that p-type dopability of ZnO can be improved through the anion substitution, replacing oxygen with other group-vi elements, such as S, Se, and Te. The band alignment between ZnO and zinc chalcogenides (ZnS, ZnSe, ZnTe) is plotted in Fig. 1 . Due to the much higher valence band of zinc chalcogenides, the acceptor activation energy is lower in the anion-substituted alloys (Zn, X = S, Se, Te), making them much more amendable to p-type doping. While the cation substitution is widely used both for the band-gap engineering (Be x O, Mg x O, and Cd x O) [56-58] and for the magnetic doping (Mn x O and Co x O) [59,60], anion substitution is much less studied, with the polycrystalline films being mostly investigated [61,62]. This is particularly surprising since this approach was previously employed to overcome problem of bipolar doping in ZnSe x Te 1-x, where high p-type and n-type levels were reported for Te-rich and Se-rich alloys, respectively [63,64]. A significant success was Fig. 1. Calculated  band alignment between ZnO and zinc chalcogenides (ZnX, X = S, Se, and Te). achieved with the so-called d-doped films where p- type dopant (N) was introduced into Te-rich nanoislands embedded within the undoped ZnSe matrix. The net acceptor concentration ([N A - N D ]) ~ 18 cm -3 was achieved in the samples containing less than 3% of Te (ZnSe 0.97 Te 0.03 ) . This is an order of magnitude higher than that achieved by any other technique. There is a report on the epitaxial growth of oxide-rich Zn (y<0.15) using PLD ; on the Se-rich side up to 1.35% of oxygen were doped in ZnO y Se 1-y [67,68]. A much larger oxygen content (x<10%) was incorporated into the ZnO x Se 1-x-y
5 30 O. Maksimov Table 5. Summary of attempts to grow anion substituted ZnO alloy. Alloy Composition (%) Growth Crystalline Bowing Reference Technique Quality Parameter(eV) ZnO y S 1-y 0 < y < 100 Sputtering Polycrystalline 3  film Zn S -y 0 < y < 100 Atomic Polycrystalline 3.6  Layer film Deposition Zn S -y 0 < y < 15 PLD Epitaxial film  ZnO y Se y 0 < y < 1.35 MBE Epitaxial film  ZnO y Se y 0 < y < 1.3 MBE Epitaxial film 8  ZnO x Se 1-x-y 0 < x < 10 MBE Epitaxial film 5 - ZnOS  9 - ZnOSe Zn 0 < y < 5 Chemical Bulk crystal 3  96 < y < 100 Vapor Transport mev to 5 mev for a heavily nitrogen doped sample . With N becoming a shallow acceptor, high p- type doping levels are much easier to achieve. Fig. 2. Band gap energy plotted vs. lattice constant for selected II-VI semiconductors. Green solid lines and black dotted lines show the estimated band gaps for Me x O and ZnO y X 1-y alloys, respectively. films closely lattice matched to GaP substrates. There, epitaxial stabilization prevented phase separation . In addition, bulk Zn (y<0.05 and y>0.96) crystals were grown using chemical vapor transport technique . All these results, summarized in Table 5, indicated a significant band gap bowing. The valance band of ZnO 0.81 S 0.19 is estimated to be 410 mev higher than that of ZnO. In this case, the acceptor activation energy decreases from ANION SUBSTITUTED ZnO FOR OPTOELECTRONIC AND PHOTOVOLTAIC DEVICES It is important to note that the band gap energy of ZnO 0.81 S 0.19 remains above 3 ev. Thus, an efficient blue emission is expected from the ZnO y S 1-y - based LEDs. In addition, an enhanced photoconductivity was observed in ZnO films co-doped with Te and nitrogen . Therefore, an enhanced performance of the UV photo detectors based on the anion substituted ZnO is also expected. With the cation substitution, band gap of the Me x O (Me = Be, Mg, Cd) can be tuned from the deep UV to the visible range of spectrum. In particular, a 2.6 ev emission line (475 nm) was observed from the Zn 0.84 Cd 0.16 O films, indicating that pure green ZnO/Cd x O LEDs can be fabricated . With the anion substitution, band gap energy of the Me x can be further adjusted throughout the whole visible range (band gap of Zn x Cd 1-x O y Se 1-y can be tuned from 3.4 to 1.7 ev) down to the near-ir region of the spectrum, (band gap of CdO x Te 1-x can decrease to ~1.1 ev assuming bowing parameter of ~3 ev). We plot band gap energies versus lattice parameters for the selected II-VI semiconductors in Fig. 2. Thus, this material is extremely promising for the fabrication of full color and pure white LEDs,
6 Recent advances and novel approaches of p-type doping of zinc oxide 31 Fig. 3. The schematics of a Cd x Te y -based multi-layer graded band gap solar cell consisting of 4 layers with decreasing energy gaps (n + -window layer with E G ~ 3.4 ev, n-absorber layer, i-absorber layer, and a p-type absorber layer with E G ~ 1.5 ev). Fig. 4. The schematics of a system based on a wide band gap Me x O y X 1-y -based solar cell and an upconverter electronically isolated from each other. Up-converter consists of a tandem of two narrow band gap solar cells, such as Ge and GaAs, driving a Me x O y X 1-y -based LED. The sub-band-gap light transmitted by the wide band gap solar cell (h < E G ) is partially up-converted into high-energy photons (h > E G ), which are subsequently absorbed by the wide band gap solar cell. A reflector is located behind the up-converter to maximize collection [79,80]. where red-green-blue emission is obtained from the heterostructures that are grown on the same substrate and differ only in the composition of the quantum well region , and photovoltaic devices, in particular, for the design of the multi-layer thin film solar cells [74-76]. In these cells, a wide band gap ZnO:Ga (E G ~3.4 ev) can be used as a transparent top n-type contact, CdTe:N can be employed as a bottom p-type contact (E G ~1.5 ev), and the layers of intermediate composition can be utilized as the absorber layers, as shown in Fig. 3. Due to the compositional gradient, multi-layer solar cells will possess the gradual reduction of the band gap and the variation of electrical conduction type from n + to p + from the front to the back. The number of layers can be increased to any number in order to absorb a major part of the solar spectrum and to produce smooth slopes of energy band edges, improving the photo-generated charge carrier separation and collection. A significant improvement in efficiency is expected for these devices since two major mecha- thermalization of high-energy photons and transmis- dition, since ZnO is already considered as a transparent top contact layer in Cu(In x Ga 1-x )Se 2 -based solar cells [77,78], such a substitution will simplify device fabrication process. Moreover, Me x -based LEDs can be epitaxially integrated with the Me x -based solar cells on the top of narrow-band gap solar cells, such as Ge/GaAs multitandem structures. In this case, two narrow band gap solar cells, absorbing low energy photons, will drive LED emitting high-
7 32 O. Maksimov energy photons. These high-energy photons will be sequentially absorbed by the electrically isolated Me x -based wide band gap solar cell in addition to the photons received directly from sun, as shown in Fig. 4. A significant improvement in the efficiency predicted for such a system [79,80] makes it extremely promising for the space applications where high efficiency is of primary importance. 4. CONCLUSION In conclusion, we reviewed recent progress in the growth of ZnO-based materials and fabrication of ZnO-based devices. We covered difficulties of doping ZnO p-type, which is known as a major obstacle for the fabrication of low turn-on-voltage light emitting and laser diodes and p-n junction photo detectors. We presented and discussed novel and extremely promising approach to achieve highly p-type doped layers via anion substitution, replacing oxygen with other group-vi elements (S, Se, and Te). We also suggested that anion substituted alloys are of particular interest for the use in the photovoltaic devices, such as highly efficient thin film solar cells. REFERENCES  U. Ozgur, Y.I. Alivov, C. Liu, A. Teke, M.A. Reschikov, S. Dogan, V. Avrutin, S.J. Cho and H. Morkoc // J. Appl. Phys. 98 (2005)  J. Muth and A. Osinsky, In: Wide Bandgap Light Emitting Materials and Devices ed. by G. F. Neumark, I. L. Kuskovsky and H. Jiang (Wiley-VCH, 2007).  B.S. Kang, H.T. Wang, L.C. Tien, F. Ren, B.P. Gila, D.P. Norton, C.R. Abernathy, J. Lin and S. J. Pearton // Sensors 6 (2006) 643.  A.B. Djurisic and Y.H. Leung // Small 2 (2006) 944.  R. Janisch, P. Gopal and N. Spaldin // J. Phys.: Condens. Matter 17 (2005) 657.  S. Ghosh, V. Sih, W.H. Lau, D. D. Awschalom, S.Y. Bae, S. Wang, S. Vaidya and G. Chapline // Appl. Phys. Lett. 86 (2007)  C.G. Van de Walle // Phys. Rev. Lett. 85 (2000)  E.C. Lee, Y.S. Kim, Y.G. Jin and K. J. Chang // Phys. Rev. B 64 (2001)  A.F. Kohan, G. Ceder, D. Morgan and C.G. Van de Walle // Phys. Rev. B 61 (2000)  L.G. Wanf and A. Zunger // Phys. Rev. Lett. 90 (2003)  T.M. Barnes, K. Olson and C.A. Wolden // Appl. Phys. Lett. 86 (2005)  X. Li, Y. Yan, T.A. Gessert, C. DeHart, C.L. Perkins, D. Young and T.J. Coutts // Electrochemical and Solid-State Lett. 6 (2003) 56.  Z.Q. Fang, B. Claflin, D.C. Look, L.L. Kerr and X. Li // J. Appl. Phys. 102 (2007)  S. Jang, J.J. Chen, B.S. Kang, F. Ren, D.P. Norton, S.J. Pearton, J. Lopata and W.S. Hobson // Appl. Phys. Lett. 87 (2005)  Z.G. Yu, P. Wu and H. Gong // Appl. Phys. Lett. 88 (2006)  Y.R. Ryu, S. Zhu, D.C. Look, J.M. Wrobel, H.M. Jeong and H.W. White // J. Crystal Growth 216 (2000) 330.  D.C. Look, G.M. Renlund, R.H. Burgener and J.R. Sizelove // Appl. Phys. Lett. 85 (2004)  V. Vaithinathan, B.T. Lee, C.W. Chang, K. Asokan and S.S. Kim // Appl. Phys. Lett. 88 (2006)  J.C. Sun, J.Z. Zhao, H.W. Liang, J.M. Bian, L.Z. Hu, H.Q. Zhang, X.P. Liang, W.F. Liu and G.T. Du // Appl. Phys. Lett. 90 (2007)  C. Yuen, S.F. Yu, E.S.P. Leong, S.P. Lau, K. Pita, H.Y. Yang and T.P. Chen // J. Appl. Phys. 101 (2007)  L.J. Mandalapu, Z. Yang, F.X. Xiu, D.T. Zhao and J.L. Liu // Appl. Phys. Lett. 88 (2006)  W. Guo, A. Allenic, Y.B. Chen, X.Q. Pan, Y. Che, Z.D. Hu and B. Liu // Appl. Phys. Lett. 90 (2007)  J.G. Lu, Y.Z. Zhang, Z.Z. Ye,Y. J. Zeng, H.P. He, L.P. Zhu, J.Y. Huang, L. Wang, J. Yuan, B.H. Zhao and X.H. Li // Appl. Phys. Lett. 89 (2006)  A. Krtschil, A. Dadgar, N. Oleynik, J. Blasing, A. Diez and A. Krost // Appl. Phys. Lett. 87 (2005)  G. Lu, Z.Z. Ye, F. Zhuge, Y.J. Zeng, B.H. Zhao and L.P. Zhu // Appl. Phys. Lett. 85 (2004)  J.G. Lu, Z.Z. Ye, G.D. Yuan, Y.J. Zeng, F. Zhuge, L.P. Zhu, B.H. Zhao and S.B. Zhang // Appl. Phys. Lett. 89 (2006)  A. Tsuzazaki, A. Ohtomo, T. Ohtomo, T. Onuma, M. Ohtani, T. Makino, M. Sumiya, K. Ohtani, S.F. Chichibu, S. Fuke,
8 Recent advances and novel approaches of p-type doping of zinc oxide 33 Y. Segawa, H. Ohno, H. Koinuma and M. Kawasaki // Nature Materials 4 (2005) 42.  H.S. Kang, B.D. Ahn, J.H. Kim, G.H. Kim, S.H. Lim, H.W. Chang and S.Y. Lee // Appl. Phys. Lett. 88 (2006)  F.X. Xiu, L.J. Mandalapu, Z. Yang, J.L. Li, G. F. Liu and J.A. Yarmoff // Appl. Phys. Lett. 89 (2006)  D.J. Rogers, F.H. Teherani, T. Monteiro, M. Soares, A. Neves, M. Carmo, S. Pereira, M.R. Correia, A. Lusson, E. Alves, N.P. Barradas, J.K. Morrod, K.A. Prior, P. Kung, A. Yasan and M. Razeghi // Phys. Stat. Sol. C 3 (2006)  M.K. Ryu, S.H. Lee, M.S. Jang, G.N. Panin and T.W. Kang // J. Appl. Phys. 92 (2002) 154.  H.F. Liu, S.J. Chua, G.X. Hu, H. Gong and N. Xiang // J. Appl. Phys. 102 (2007)  S. Yu. Yuldashev, G.N. Panin, S.W. Choi, V.Sh. Yalishev, L.A. Nosova, M.K. Ryu, S. Lee, M.S. Jang, K.S. Chung and T.W. Kang // Jpn. J. Appl. Phys. 42 (2003)  S. Limpijumnong, S.B. Zhang, S.H. Wei and C.H. Park // Phys. Rev. Lett. 92 (2004)  H. Ohta, M. Orita, M. Hirano and H. Hosono // J. Appl. Phys. 89 (2001)  C. Yuen, S.F. Yu, S.P. Lau, Rusli and T.P. Chen // Appl. Phys. Lett. 86 (2005)  P. Chen, X. Ma and D. Yang // J. Appl. Phys. 101 (2007)  D.K. Hwang, M.S. Oh, J.H. Lim, Y.S. Choi and S.J. Park // Appl. Phys. Lett. 91 (2007)  S.J. Ahn and G.C. Yi // Appl. Phys. Lett. 91 (2007)  Y.I. Alivov, J.E. Van Nostrand, D.C. Look, M.V. Chukichev and B.M. Ataev // Appl. Phys. Lett. 83 (2003)  D.J. Rogers, F.H. Teherani, A. Yasan, K. Minder, P. Kung and M. Razeghi // Appl. Phys. Lett. 88 (2006)  J.W. Osinsky, M.Z. Dong, B. Kauser, A. Hertog, M. Dabiran, P.P. Chow, S.J. Pearton, O. Lopatiuk and L. Chernyak // Appl. Phys. Lett. 85 (2004)  S.J. Jiao, Z.Z. Zhang, Y.M. Lu, D.Z. Shen, B. Yao, J.Y. Zhang, B.H. Li, D.X. Zhao, X.W. Fan and Z.K. Tang // Appl. Phys. Lett. 88 (2006)  Y. Ryu, T. Lee, J.A. Lubdugan, H.W. White, B.J. Kim, Y.S. Park and C.J. Youn // Appl. Phys. Lett. 88 (2006)  Z.Z. Zhang, Z.P. Wei, Y.M. Lu, D.Z. Shen, B.Yao, B.H. Li, D.X. Zhao, J.Y. Zhang, X.W. Fan and Z.K. Tang // J. Crystal Growth 301 (2007) 362.  J.C. Sun, J.Z. Zhao, H.W. Liang, J.M. Bian, L.Z. Hu, H.Q. Zhang, X.P. Liang, W.F. Liu and G.T. Du // Appl. Phys. Lett. 90 (2007).  A. Tsuzazaki, A. Ohtomo, T. Ohtomo, T. Onuma, M. Ohtani, T. Makino, M. Sumiya, K. Ohtani, S.F. Chichibu, S. Fuke, Y. Segawa, H. Ohno, H. Koinuma and M. Kawasaki // Nature Materials 4 (2005) 42.  J. Bian, W. Liu, H. Liang, L. Hu, J. Sun, Y. Luo and G. Du // Chem. Phys. Lett. 430 (2006) 183.  W. Yang, R.D. Vispute, S. Choopun, R.P. Sharma, T. Venkatesan and H. Shen // Appl. Phys. Lett. 78 (2001)  W. Yang, S.S. Hullavarad, B. Nagaraj, I. Takeuchi, R.P. Sharma, T. Venkatesan, R.D. Vispute and H. Shen // Appl. Phys. Lett. 82 (2003)  K.W. Liu, J.Y. Zhang, J.G. Ma, D.Y. Jiang, Y.M. Lu, B. Yao, B.H. Li, D.X. Zhao, Z.Z. Zhang and D.Z. Shen // J. Phys. D 40 (2007)  K. Tamura, A. Ohtomo, K. Saikusa, Y. Osaka, T. Makino, Y. Segawa, M. Sumiya, S. Fuke, H. Koinuma and M. Kawasaki // J. Crystal Growth 214 (2000) 59.  B.J. Kwon, H.S. Kwack, S.K. Lee, Y.H. Cho, D.K. Hwang and S.J. Park // Appl. Phys. Lett. 91 (2007)  W. Guo, A. Allenic, Y.B. Chen, X.Q. Pan, Y. Che, Z.D. Hu and B. Liu // Appl. Phys. Lett. 90 (2007)  S.H. Wei and A. Zunger // Appl. Phys. Lett. 72 (1998)  Y.R. Ryu, T.S. Lee, J.A. Lubguban, A.B. Corman, H.W. White, J.H. Leem, M.S. Han, Y.S. Park, C.J. Youn and W.J. Kim // Appl. Phys. Lett. 88 (2006)  A. Ohtomo, M. Kawasaki, T. Koida, K. Masubuchi, H. Koinuma, Y. Sakurai, Y. Yoshida, T. Yasuda and Y. Segawa // Appl. Phys. Lett. 72 (1998)  S.Y. Lee, Y. Li, J.S. Lee, J.K. Lee, M. Nastasi, S.A. Crooker, Q.X. Jia, H.S. Kang and J.S. Kang // Mat. Res. Soc. Symp. Proc. 764 (2003) 413.
9 34 O. Maksimov  Z. Jin, M. Murakami, T. Fukumura, Y. Matsumoto, A. Ohtomo, M. Kawasaki and H. Koinuma // J. Crystal Growth 214 (2000) 55.  T. Fukumura, Z. Jin, A. Ohtomo, H. Koinuma and M. Kawasaki // Appl. Phys. Lett. 75 (1999)  B.K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kramer and C. Wang // Appl. Phys. Lett. 85 (2004)  C. Persson, C. Platzer-Bjorkman, J. Malmstrom, T. Torndahl and M. Edoff // Phys. Rev. Lett. 97 (2006)  W. Lin, B.X. Yang, S.P. Guo, A. Elmoumni, F. Fernandez and M.C. Tamargo // Appl. Phys. Lett. 75 (2007)  M. Strassburg, M. Strassburg, O. Schulz, U. Pohl, A. Hoffmann, D. Bimberg, A. Kontos and Y. Raptis // J. Crystal Growth 248 (2003) 50.  I.L. Kuskovsky, Y. Gu, Y. Gong, H.F. Yan, J. Lau, I.C. Noyan, G.F. Neumark, O. Maksimov, X. Zhou, M.C. Tamargo, V. Volkov, Y. Zhu and L. Wang // Phys. Rev. B 73 (2006)  Y.Z. Yoo, Z.W. Jin, T. Chikyow, T. Fukumura, M. Kawasaki and H. Koinuma // Appl. Phys. Lett. 81 (2002)  W. Shan, W. Walukiewicz, J.W. Ager III, K.M. Yu, J. Wu, E.E. Haller, Y. Nabetani, T. Mukawa, Y. Ito and T. Matsumoto // Appl. Phys. Lett. 83 (2003) 299.  Y. Nabetani, T. Mukawa, Y. Ito, T. Kato and T. Matsumoto // Appl. Phys. Lett. 83 (2003)  Y. Nabetani, Y. Ito, K. Kamisawa, T. Kato, T. Matsumoto and T. Hirai // Phys. Stat. Sol. C 3 (2006)  S. Locmelis, C. Brunig, M. Binnewies, A. Borger, K.D. Becker. T. Homann and T. Bredow // J. Mater. Sci. 42 (2007)  H.L. Porter, A.L. Cai, J.F. Muth and J. Narayan // Appl. Phys. Lett. 86 (2005)  I.A. Buyanova, J.P. Bergman, G. Pozina, W.M. Chen, S. Rawal, D.P. Norton, S.J. Pearton, A. Osinsky and J.W. Dong // Appl. Phys. Lett. 90 (2007)  Y. Luo, S.P. Guo, O. Maksimov, M.C. Tamargo, V. Asnin, F.H. Pollak and Y.C. Chen // Appl. Phys. Lett. 77 (2000)  N.B. Chaure, A.P. Samantilleke, R.P. Burton, J. Young and I.M. Dharmadasa // Thin Solid Films 472 (2005) 212.  I.M. Dharmasada // Solar Energy Materials & Solar Cells 85 (2005) 293.  I.M. Dharmadasa, J.S. Roberts and G. Hill // Solar Energy Materials & Solar Cells 88 (2005) 413.  F.J. Haug, M. Krejci, H. Zogg, A.N. Tiwari, M. Kirsch and S. Siebentritt // Thin Solid Films 361 (2000) 239.  P.J. Rostan, J. Mattheis, G. Bilger, U. Rau and J.H. Werner // Thin Solid Films 480 (2005) 67.  T. Trupke, M.A. Green and P. Wurfel // J. Appl. Phys. 92 (2002)  P. Wurfel, Physics of Solar Cells (Wiley- VCH, New York, 2007).  A. Ohtomo, K. Tamura, K. Saikusa, K. Takahashi, T. Makino, Y. Segawa, H. Koinuma and M. Kawasaki // Appl. Phys. Lett. 75 (1999)  H.J. Ko, Y.F. Chen, T. Yao, K. Miyajima, A. Yamamoto and T. Goto // Appl. Phys. Lett. 77 (2000) 537.